The material structure described by Li5Ti2V3O10 is Caswellsilverite-derived structured and crystallizes in the triclinic P-1 space group. There are three inequivalent Li sites. In the first Li site, Li(1) is bonded to two equivalent O(2), two equivalent O(4), and two equivalent O(5) atoms to form LiO6 octahedra that share corners with two equivalent Li(2)O6 octahedra, corners with two equivalent Li(3)O6 octahedra, corners with two equivalent V(1)O6 octahedra, edges with two equivalent Li(3)O6 octahedra, edges with two equivalent V(2)O6 octahedra, edges with four equivalent Li(2)O6 octahedra, and edges with four equivalent Ti(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 6-12°. In the second Li site, Li(2) is bonded to one O(1), one O(4), two equivalent O(2), and two equivalent O(5) atoms to form LiO6 octahedra that share  a cornercorner with one Li(1)O6 octahedra, corners with two equivalent Ti(1)O6 octahedra, corners with three equivalent V(2)O6 octahedra,  an edgeedge with one V(1)O6 octahedra,  an edgeedge with one V(2)O6 octahedra, edges with two equivalent Li(1)O6 octahedra, edges with two equivalent Li(2)O6 octahedra, edges with three equivalent Li(3)O6 octahedra, and edges with three equivalent Ti(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 1-11°. In the third Li site, Li(3) is bonded to one O(1), one O(2), one O(4), one O(5), and two equivalent O(3) atoms to form LiO6 octahedra that share  a cornercorner with one Li(1)O6 octahedra, corners with two equivalent V(2)O6 octahedra, corners with three equivalent Ti(1)O6 octahedra,  an edgeedge with one Li(1)O6 octahedra,  an edgeedge with one Li(3)O6 octahedra, edges with two equivalent Ti(1)O6 octahedra, edges with two equivalent V(1)O6 octahedra, edges with three equivalent Li(2)O6 octahedra, and edges with three equivalent V(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 1-12°. Ti(1) is bonded to one O(1), one O(3), one O(4), one O(5), and two equivalent O(2) atoms to form TiO6 octahedra that share  a cornercorner with one V(1)O6 octahedra, corners with two equivalent Li(2)O6 octahedra, corners with three equivalent Li(3)O6 octahedra,  an edgeedge with one Ti(1)O6 octahedra,  an edgeedge with one V(1)O6 octahedra, edges with two equivalent Li(1)O6 octahedra, edges with two equivalent Li(3)O6 octahedra, edges with three equivalent Li(2)O6 octahedra, and edges with three equivalent V(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 4-10°. There are two inequivalent V sites. In the first V site, V(1) is bonded to two equivalent O(1), two equivalent O(3), and two equivalent O(4) atoms to form VO6 octahedra that share corners with two equivalent Li(1)O6 octahedra, corners with two equivalent Ti(1)O6 octahedra, corners with two equivalent V(2)O6 octahedra, edges with two equivalent Li(2)O6 octahedra, edges with two equivalent Ti(1)O6 octahedra, edges with four equivalent Li(3)O6 octahedra, and edges with four equivalent V(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 4-8°. In the second V site, V(2) is bonded to one O(4), one O(5), two equivalent O(1), and two equivalent O(3) atoms to form VO6 octahedra that share  a cornercorner with one V(1)O6 octahedra, corners with two equivalent Li(3)O6 octahedra, corners with three equivalent Li(2)O6 octahedra,  an edgeedge with one Li(1)O6 octahedra,  an edgeedge with one Li(2)O6 octahedra, edges with two equivalent V(1)O6 octahedra, edges with two equivalent V(2)O6 octahedra, edges with three equivalent Li(3)O6 octahedra, and edges with three equivalent Ti(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 1-11°. There are five inequivalent O sites. In the first O site, O(1) is bonded to one Li(2), one Li(3), one Ti(1), one V(1), and two equivalent V(2) atoms to form OLi2TiV3 octahedra that share  a cornercorner with one O(1)Li2TiV3 octahedra,  a cornercorner with one O(3)Li2TiV3 octahedra,  a cornercorner with one O(4)Li3TiV2 octahedra,  a cornercorner with one O(2)Li4Ti2 octahedra, corners with two equivalent O(5)Li4TiV octahedra,  an edgeedge with one O(1)Li2TiV3 octahedra, edges with two equivalent O(2)Li4Ti2 octahedra, edges with two equivalent O(5)Li4TiV octahedra, edges with three equivalent O(4)Li3TiV2 octahedra, and edges with four equivalent O(3)Li2TiV3 octahedra. The corner-sharing octahedral tilt angles range from 0-9°. In the second O site, O(2) is bonded to one Li(1), one Li(3), two equivalent Li(2), and two equivalent Ti(1) atoms to form OLi4Ti2 octahedra that share  a cornercorner with one O(1)Li2TiV3 octahedra,  a cornercorner with one O(4)Li3TiV2 octahedra,  a cornercorner with one O(2)Li4Ti2 octahedra,  a cornercorner with one O(5)Li4TiV octahedra, corners with two equivalent O(3)Li2TiV3 octahedra,  an edgeedge with one O(3)Li2TiV3 octahedra, edges with two equivalent O(1)Li2TiV3 octahedra, edges with two equivalent O(2)Li4Ti2 octahedra, edges with three equivalent O(4)Li3TiV2 octahedra, and edges with four equivalent O(5)Li4TiV octahedra. The corner-sharing octahedral tilt angles range from 0-11°. In the third O site, O(3) is bonded to two equivalent Li(3), one Ti(1), one V(1), and two equivalent V(2) atoms to form OLi2TiV3 octahedra that share  a cornercorner with one O(1)Li2TiV3 octahedra,  a cornercorner with one O(3)Li2TiV3 octahedra,  a cornercorner with one O(4)Li3TiV2 octahedra,  a cornercorner with one O(5)Li4TiV octahedra, corners with two equivalent O(2)Li4Ti2 octahedra,  an edgeedge with one O(2)Li4Ti2 octahedra, edges with two equivalent O(3)Li2TiV3 octahedra, edges with two equivalent O(5)Li4TiV octahedra, edges with three equivalent O(4)Li3TiV2 octahedra, and edges with four equivalent O(1)Li2TiV3 octahedra. The corner-sharing octahedral tilt angles range from 0-11°. In the fourth O site, O(4) is bonded to one Li(1), one Li(2), one Li(3), one Ti(1), one V(1), and one V(2) atom to form OLi3TiV2 octahedra that share  a cornercorner with one O(1)Li2TiV3 octahedra,  a cornercorner with one O(3)Li2TiV3 octahedra,  a cornercorner with one O(2)Li4Ti2 octahedra,  a cornercorner with one O(5)Li4TiV octahedra, corners with two equivalent O(4)Li3TiV2 octahedra, edges with three equivalent O(1)Li2TiV3 octahedra, edges with three equivalent O(3)Li2TiV3 octahedra, edges with three equivalent O(2)Li4Ti2 octahedra, and edges with three equivalent O(5)Li4TiV octahedra. The corner-sharing octahedral tilt angles range from 0-11°. In the fifth O site, O(5) is bonded to one Li(1), one Li(3), two equivalent Li(2), one Ti(1), and one V(2) atom to form OLi4TiV octahedra that share  a cornercorner with one O(3)Li2TiV3 octahedra,  a cornercorner with one O(4)Li3TiV2 octahedra,  a cornercorner with one O(2)Li4Ti2 octahedra,  a cornercorner with one O(5)Li4TiV octahedra, corners with two equivalent O(1)Li2TiV3 octahedra,  an edgeedge with one O(5)Li4TiV octahedra, edges with two equivalent O(1)Li2TiV3 octahedra, edges with two equivalent O(3)Li2TiV3 octahedra, edges with three equivalent O(4)Li3TiV2 octahedra, and edges with four equivalent O(2)Li4Ti2 octahedra. The corner-sharing octahedral tilt angles range from 0-11°. is represented by the CIF card [CIF]
data_Li5Ti2V3O10
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   5.147
_cell_length_b   5.191
_cell_length_c   7.834
_cell_angle_alpha   108.628
_cell_angle_beta   107.949
_cell_angle_gamma   81.008
_symmetry_Int_Tables_number   1
_cell_volume   188.308
_cell_formula_units_Z   1
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  Li  Li0  1  0.004  0.500  0.503  1.0
  Li  Li1  1  0.507  0.218  0.409  1.0
  Li  Li2  1  0.501  0.779  0.597  1.0
  Li  Li3  1  0.481  0.397  0.783  1.0
  Li  Li4  1  0.526  0.601  0.223  1.0
  O  O5  1  0.754  0.042  0.849  1.0
  O  O6  1  0.254  0.956  0.158  1.0
  O  O7  1  0.222  0.137  0.543  1.0
  O  O8  1  0.786  0.861  0.463  1.0
  O  O9  1  0.249  0.330  0.935  1.0
  O  O10  1  0.760  0.668  0.072  1.0
  O  O11  1  0.757  0.221  0.246  1.0
  O  O12  1  0.251  0.777  0.760  1.0
  O  O13  1  0.768  0.426  0.662  1.0
  O  O14  1  0.239  0.572  0.344  1.0
  Ti  Ti15  1  0.985  0.106  0.696  1.0
  Ti  Ti16  1  0.023  0.893  0.311  1.0
  V  V17  1  0.504  0.999  0.003  1.0
  V  V18  1  0.009  0.696  0.907  1.0
  V  V19  1  1.000  0.302  0.100  1.0
[/CIF]
.
The material structure described by Li5Ti2V3O10 is Caswellsilverite-derived structured and crystallizes in the triclinic P-1 space group. There are three inequivalent Li sites. In the first Li site, Li(1) is bonded to two equivalent O(2), two equivalent O(4), and two equivalent O(5) atoms to form LiO6 octahedra that share corners with two equivalent Li(2)O6 octahedra, corners with two equivalent Li(3)O6 octahedra, corners with two equivalent V(1)O6 octahedra, edges with two equivalent Li(3)O6 octahedra, edges with two equivalent V(2)O6 octahedra, edges with four equivalent Li(2)O6 octahedra, and edges with four equivalent Ti(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 6-12°. In the second Li site, Li(2) is bonded to one O(1), one O(4), two equivalent O(2), and two equivalent O(5) atoms to form LiO6 octahedra that share  a cornercorner with one Li(1)O6 octahedra, corners with two equivalent Ti(1)O6 octahedra, corners with three equivalent V(2)O6 octahedra,  an edgeedge with one V(1)O6 octahedra,  an edgeedge with one V(2)O6 octahedra, edges with two equivalent Li(1)O6 octahedra, edges with two equivalent Li(2)O6 octahedra, edges with three equivalent Li(3)O6 octahedra, and edges with three equivalent Ti(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 1-11°. In the third Li site, Li(3) is bonded to one O(1), one O(2), one O(4), one O(5), and two equivalent O(3) atoms to form LiO6 octahedra that share  a cornercorner with one Li(1)O6 octahedra, corners with two equivalent V(2)O6 octahedra, corners with three equivalent Ti(1)O6 octahedra,  an edgeedge with one Li(1)O6 octahedra,  an edgeedge with one Li(3)O6 octahedra, edges with two equivalent Ti(1)O6 octahedra, edges with two equivalent V(1)O6 octahedra, edges with three equivalent Li(2)O6 octahedra, and edges with three equivalent V(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 1-12°. Ti(1) is bonded to one O(1), one O(3), one O(4), one O(5), and two equivalent O(2) atoms to form TiO6 octahedra that share  a cornercorner with one V(1)O6 octahedra, corners with two equivalent Li(2)O6 octahedra, corners with three equivalent Li(3)O6 octahedra,  an edgeedge with one Ti(1)O6 octahedra,  an edgeedge with one V(1)O6 octahedra, edges with two equivalent Li(1)O6 octahedra, edges with two equivalent Li(3)O6 octahedra, edges with three equivalent Li(2)O6 octahedra, and edges with three equivalent V(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 4-10°. There are two inequivalent V sites. In the first V site, V(1) is bonded to two equivalent O(1), two equivalent O(3), and two equivalent O(4) atoms to form VO6 octahedra that share corners with two equivalent Li(1)O6 octahedra, corners with two equivalent Ti(1)O6 octahedra, corners with two equivalent V(2)O6 octahedra, edges with two equivalent Li(2)O6 octahedra, edges with two equivalent Ti(1)O6 octahedra, edges with four equivalent Li(3)O6 octahedra, and edges with four equivalent V(2)O6 octahedra. The corner-sharing octahedral tilt angles range from 4-8°. In the second V site, V(2) is bonded to one O(4), one O(5), two equivalent O(1), and two equivalent O(3) atoms to form VO6 octahedra that share  a cornercorner with one V(1)O6 octahedra, corners with two equivalent Li(3)O6 octahedra, corners with three equivalent Li(2)O6 octahedra,  an edgeedge with one Li(1)O6 octahedra,  an edgeedge with one Li(2)O6 octahedra, edges with two equivalent V(1)O6 octahedra, edges with two equivalent V(2)O6 octahedra, edges with three equivalent Li(3)O6 octahedra, and edges with three equivalent Ti(1)O6 octahedra. The corner-sharing octahedral tilt angles range from 1-11°. There are five inequivalent O sites. In the first O site, O(1) is bonded to one Li(2), one Li(3), one Ti(1), one V(1), and two equivalent V(2) atoms to form OLi2TiV3 octahedra that share  a cornercorner with one O(1)Li2TiV3 octahedra,  a cornercorner with one O(3)Li2TiV3 octahedra,  a cornercorner with one O(4)Li3TiV2 octahedra,  a cornercorner with one O(2)Li4Ti2 octahedra, corners with two equivalent O(5)Li4TiV octahedra,  an edgeedge with one O(1)Li2TiV3 octahedra, edges with two equivalent O(2)Li4Ti2 octahedra, edges with two equivalent O(5)Li4TiV octahedra, edges with three equivalent O(4)Li3TiV2 octahedra, and edges with four equivalent O(3)Li2TiV3 octahedra. The corner-sharing octahedral tilt angles range from 0-9°. In the second O site, O(2) is bonded to one Li(1), one Li(3), two equivalent Li(2), and two equivalent Ti(1) atoms to form OLi4Ti2 octahedra that share  a cornercorner with one O(1)Li2TiV3 octahedra,  a cornercorner with one O(4)Li3TiV2 octahedra,  a cornercorner with one O(2)Li4Ti2 octahedra,  a cornercorner with one O(5)Li4TiV octahedra, corners with two equivalent O(3)Li2TiV3 octahedra,  an edgeedge with one O(3)Li2TiV3 octahedra, edges with two equivalent O(1)Li2TiV3 octahedra, edges with two equivalent O(2)Li4Ti2 octahedra, edges with three equivalent O(4)Li3TiV2 octahedra, and edges with four equivalent O(5)Li4TiV octahedra. The corner-sharing octahedral tilt angles range from 0-11°. In the third O site, O(3) is bonded to two equivalent Li(3), one Ti(1), one V(1), and two equivalent V(2) atoms to form OLi2TiV3 octahedra that share  a cornercorner with one O(1)Li2TiV3 octahedra,  a cornercorner with one O(3)Li2TiV3 octahedra,  a cornercorner with one O(4)Li3TiV2 octahedra,  a cornercorner with one O(5)Li4TiV octahedra, corners with two equivalent O(2)Li4Ti2 octahedra,  an edgeedge with one O(2)Li4Ti2 octahedra, edges with two equivalent O(3)Li2TiV3 octahedra, edges with two equivalent O(5)Li4TiV octahedra, edges with three equivalent O(4)Li3TiV2 octahedra, and edges with four equivalent O(1)Li2TiV3 octahedra. The corner-sharing octahedral tilt angles range from 0-11°. In the fourth O site, O(4) is bonded to one Li(1), one Li(2), one Li(3), one Ti(1), one V(1), and one V(2) atom to form OLi3TiV2 octahedra that share  a cornercorner with one O(1)Li2TiV3 octahedra,  a cornercorner with one O(3)Li2TiV3 octahedra,  a cornercorner with one O(2)Li4Ti2 octahedra,  a cornercorner with one O(5)Li4TiV octahedra, corners with two equivalent O(4)Li3TiV2 octahedra, edges with three equivalent O(1)Li2TiV3 octahedra, edges with three equivalent O(3)Li2TiV3 octahedra, edges with three equivalent O(2)Li4Ti2 octahedra, and edges with three equivalent O(5)Li4TiV octahedra. The corner-sharing octahedral tilt angles range from 0-11°. In the fifth O site, O(5) is bonded to one Li(1), one Li(3), two equivalent Li(2), one Ti(1), and one V(2) atom to form OLi4TiV octahedra that share  a cornercorner with one O(3)Li2TiV3 octahedra,  a cornercorner with one O(4)Li3TiV2 octahedra,  a cornercorner with one O(2)Li4Ti2 octahedra,  a cornercorner with one O(5)Li4TiV octahedra, corners with two equivalent O(1)Li2TiV3 octahedra,  an edgeedge with one O(5)Li4TiV octahedra, edges with two equivalent O(1)Li2TiV3 octahedra, edges with two equivalent O(3)Li2TiV3 octahedra, edges with three equivalent O(4)Li3TiV2 octahedra, and edges with four equivalent O(2)Li4Ti2 octahedra. The corner-sharing octahedral tilt angles range from 0-11°. is represented by the CIF card [CIF]
data_Li5Ti2V3O10
_symmetry_space_group_name_H-M   'P 1'
_cell_length_a   5.147
_cell_length_b   5.191
_cell_length_c   7.834
_cell_angle_alpha   108.628
_cell_angle_beta   107.949
_cell_angle_gamma   81.008
_symmetry_Int_Tables_number   1
_cell_volume   188.308
_cell_formula_units_Z   1
loop_
 _symmetry_equiv_pos_site_id
 _symmetry_equiv_pos_as_xyz
  1  'x, y, z'
loop_
 _atom_site_type_symbol
 _atom_site_label
 _atom_site_symmetry_multiplicity
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_occupancy
  Li  Li0  1  0.004  0.500  0.503  1.0
  Li  Li1  1  0.507  0.218  0.409  1.0
  Li  Li2  1  0.501  0.779  0.597  1.0
  Li  Li3  1  0.481  0.397  0.783  1.0
  Li  Li4  1  0.526  0.601  0.223  1.0
  O  O5  1  0.754  0.042  0.849  1.0
  O  O6  1  0.254  0.956  0.158  1.0
  O  O7  1  0.222  0.137  0.543  1.0
  O  O8  1  0.786  0.861  0.463  1.0
  O  O9  1  0.249  0.330  0.935  1.0
  O  O10  1  0.760  0.668  0.072  1.0
  O  O11  1  0.757  0.221  0.246  1.0
  O  O12  1  0.251  0.777  0.760  1.0
  O  O13  1  0.768  0.426  0.662  1.0
  O  O14  1  0.239  0.572  0.344  1.0
  Ti  Ti15  1  0.985  0.106  0.696  1.0
  Ti  Ti16  1  0.023  0.893  0.311  1.0
  V  V17  1  0.504  0.999  0.003  1.0
  V  V18  1  0.009  0.696  0.907  1.0
  V  V19  1  1.000  0.302  0.100  1.0
[/CIF]
.